Quantitative Analysis Reference Intensity Ratio (RIR). Reference Intensity Ratio (RIR) What is it?. The Reference Intensity Ratio (RIR) is a method used for Quantitative Analysis by Powder Diffraction.
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
The Reference Intensity Ratio (RIR) is a method used for Quantitative Analysis by Powder Diffraction.
The RIR method is based upon scaling all diffraction data to the diffraction of standard reference materials.
The intensity of a diffraction peak profile is a convolution of
many factors, only one of which is the concentration of the
analyte (species being measured).
By using the RIR method, ratios scaled to a common reference, are used in the experiment. The assumption is that all the factors, except concentration, of the analyte are ratioed and reduced to a constant.
By using ratios and measuring peak areas, the RIR method can be used to determine concentrations.
The RIR method scales all diffraction data to a standard.
By convention, corundum is used as the international reference and the scale factor is defined by:
Intensity Analyte / Intensity Corundum = I / Ic
I/Ic can be experimentally derived by adding a known weight
fraction of corundum to a pure specimen of the analyte of interest.
I/Ic can also be calculated if the atomic parameters of analyte
are known because the atomic parameters of corundum have been determined.
In PDF-4+, I/Ic has been experimentally determined for close to 10,000 materials and has been calculated for >170,000 materials.
To understand how to use I/Ic values for quantitative analysis with the PDF-4+ database, a short description of the method is provided in the following slides.
RIR, as used in the Powder Diffraction File, is I/Ic (reference to corundum).
I/Ic can be determined, experimentally or calculated, from a crystal structure, both methods are used in the PDF-4+ database.
Experimentally, I/Ic can be determined by taking
the ratio of the strongest line of the pattern to the intensity of the strongest line of corundum in a 50/50 weight mixture.
If we know the crystal structure, we can calculate I/Ic as shown in the following slide.
All calculated patterns have I/Ic.
I/Ic = c /c c
= Linear attenuation coefficient
= Absolute scale factor
(Subscript “c” corresponds to corundum)
Single crystal determinations have all the data necessary to calculate the variables in the above equation from atomic parameters and the unit cell parameters with the use of atomic scattering factors and published constants. These are used by
the ICDD to calculate I/Ic for these entries.
Calculated I/Ic values often significantly differ from
experimental I/Ic values.
Natural products, minerals, and biomaterials often contain trace impurities, anion/cation substitution in the lattice, or naturally produced vacancies, and/or defects in the crystalline state. These physical phenomena are well known to influence peak intensities and peak profiles that will change the I/c value. This value can be significantly different from one calculated from a perfect crystalline pure material.
If you are using I/Ic to quantitate a synthetic mixture, you may want to use a calculated value. If you are using I/Ic to quantitate a natural product or mineral sample, you may prefer experimental values.
Iia = intensity of reflection i of phase a
Mainequation for quantitative analysis
Kia contains structure factor,
factor, temperature factor +
scale factor for reflection i of
Xa = wt fraction of
phase a (want this!!)
= Linear attenuation coefficient
a is density
of phase a
Xa = wt fraction of phase a (want this!!)
For 50-50 mixture of analyte with corundum
K …..denoted (I/Ic)a
Quantitative AnalysisReference Intensity Ratios
Quantitative AnalysisReference Intensity Ratios
For any a + b mixture
The RIR method uses simultaneous equations to solve analyte concentrations in a multicomponent mixture.
Many vendor programs interface to PDF-4+ to automatically extract I/Ic and peak areas from the experimental data for automated quantitative analysis.
Automated programs assume that the combination of all phases identified account for all observed scattering and 100% of the specimen. Significant errors can occur, if there are non-crystalline phases or unidentified materials present in the specimen.
Start at the main
Go to the
1) Perform a Search
2) Select the Preferences Tab
3) Select I/Ic to display Values
Choose the appropriate structure.
Many materials have polymorphs that have the same chemical formula, but different
structures. These have different I/Ic’s.
Match the reference to the specimen as closely as possible.
Use quality marks and indicators to select
the best quality reference.
I/Ic = 3.54
I/Ic = 3.06
Formulae are the same,
pattern, structure and I/Ic
are distinctly different
I/Ic = 5.04
You can select many fields that
help you determine the structure
by matching these data to the experimental data.
Chemical Name, Mineral Name
System and Space Group Number
Pearson, Prototype Structure and
LPF Prototype Structure
Reduced Cell, Author Cell and
Strong Line (D1, D2, D3) and
Long Line (L1, L2, L3)
From Search Results
use the Preferences Tab
to select fields
expand or contract
the unit cell – and
All the known factors that can alter a structure: temperature, pressure, anion or cation substitution, synthesis conditions, vacancies, stress, strain, etc. will change atom positions, electron density distribution, and therefore alter peak intensities and the I/Ic ratio.
The above factors are changes in the Kia factor in the equation for quantitative analysis.
Select a reference that most closely matches your experiment!
From the Results Form,
add Database Comments
Editor comments contain information on specimen preparation,
impurities, temperature of data collection and other factors that
can change I/Ic. They can guide you to the appropriate choice.
Data plotted from
PDF-4+ Search Form
of I/Ic versus reduced
cell a, editor comments
describe T, P conditions
Effect of Temp and Pressure
for Quartz I/Ic
High Pressure Series
The database contains many quality
Indicators. These include:
Indicator High Quality Value
Quality Mark S
SS/FOM Highest Number
R-Factor Lowest Number
Database Comments: This includes
comments from editors and statistical
analyses conducted on the data.
The indicators are defined in the
Help documentation in the database.
Use “Preferences” to display quality marks and indicators.
Low Quality Marks are designations B and O
Low Quality Status would be a “Deleted” pattern
R-factors >0.10 (i.e., 10%) and SS/FOM’s below 10 are
indications of poor quality
In general, any data meeting the above criteria should not be used in a quantitative analysis calculation as the ICDD’s editorial analysis and review would indicate that the calculation may result in large errors.
The data are included because there may not be better alternative choices for a particular material or the entry may contain other types of unique data (i.e., measured physical properties, novel synthesis, etc.).
What if a Search/Match program identified an entry with a poor quality mark or poor quality indicator?
- Check the Cross References
In this example, a Search/Match program
identified entry PDF 04-08-7810, which has
an I/Ic of 3.6 and a “B” Quality Mark. The editors’ comments mention that the atomic
parameters were derived (not experimentally
determined or calculated) from the original
publication. This results in low precision for
the cell parameters and I/Ic values.
Solution: The entry contains cross-
references identified in the “Miscellaneous
Tab” of the entry. The primary (high quality)
entry is highlighted and is an active link in
the database. The primary entry has an I/Ic of 3.61 and is an “S” quality entry.
Using ICDD’s SIeve and SIeve+ programs, materials are identified, peak intensities of each phase are calculated and I/Ic values are displayed – allowing the user to calculate concentrations by the RIR method.
Many software distributors have RIR calculation modules, which can perform multiple, simultaneous calculations for complex mixtures, use integrated intensities and correct for absorption – all in a matter of seconds!
Examples are shown for the above.
Two phase identification
in the analysis of an
This results in 96% magnesium aluminum silicate and
4% cerium zirconium oxide and uses peak intensities.
This software calculated 92% magnesium aluminum silicate and 7% cerium zirconium oxide using integrated intensities.
Thank you for viewing our tutorial. Additional tutorials are available at the ICDD website (www.icdd.com).
International Centre for Diffraction Data
12 Campus Boulevard
Newtown Square, PA 19073